Materials and Design 29 (2008) Delamination in FRP laminates with holes under transverse impact. Tarapada Roy, Debabrata Chakraborty *


 Shanon Morris
 1 years ago
 Views:
Transcription
1 Materials and Design 9 (8) Materials & Design Delamination in FRP laminates with holes under transverse impact Tarapada Roy, Debabrata Chakraborty * Mechanical Engineering Department, Indian Institute of Technology Guwahati , Assam, India Received 4 July 6; accepted 14 November 6 Available online 16 January 7 Abstract The present paper deals with the study of hybridization on impact response and impact induced delamination of laminated composite plates with holes. Three dimensional finite element analysis has been done to evaluate the response of graphite/epoxy laminate as well as graphite/epoxy kevlar/epoxy hybrid laminate subjected to impact loading, and stress based delamination criterion has been used to assess the chances of delamination initiation from the inner edges of the hole at different interfaces. The present study concludes that incorporation of kevlar/epoxy at the outer layers of the [/ 45/45/9] S in the graphite/epoxy laminate improves the impact resistance of the laminate in terms of reduced magnitude of the contact force but the chances of impact induced delamination at the interfaces increase. Ó 6 Elsevier Ltd. All rights reserved. Keywords: Hybrid laminate; Finite element; Delamination; Contact impact 1. Introduction Inherent advantages like high specific weight and stiffness of fiber reinforced polymer (FRP) composites led to its extensive use in aerospace and allied industries. However, in spite of their having many advantages, the structures made of FRP composites are susceptible to transverse impact. Especially in the case of low velocity impact, damages such as matrix cracking, fiber breakage and delamination occur at certain specific plies in the laminate depending upon the stacking sequence as well as the strength of the plies leading to embedded defects which are not apparent. Many a times the laminated composite plates contain holes due to various reasons like accommodating bolted joints or other mating parts in the structures. The presence of such holes in a laminate gives rise to free edges around the inner circumference of the hole. Subjected to loading, interlaminar stresses develop at these free edges and delamination may initiate depending upon the strength of the interface. Once a defect of this kind occurs in a laminated structure, * Corresponding author. Tel.: ; fax: address: (D. Chakraborty). failure initiates from that location leading to the final fracture of the laminate. Many investigations have been performed to study the response of laminated composites under low velocity impact and the approaches to improve the impact resistance of laminated composites. Hybridization has been one of the ways to improve the impact resistance of the laminated composites. Experimental and numerical studies have been conducted to study the improvement of impact response of laminated composites by way of hybridization. Some of the important works in this direction are presented in the following paragraph. Sun and Chattopadhyay [1] investigated the impact of a mass on a simply supported composite plate under initial stress by solving a nonlinear integral equation and obtained the contact force and dynamic response of the plate. Sun and Chen [] analyzed the impact response behavior of initially stressed composite plate. Wu et al. [3] performed a transient dynamic finite element analysis of a laminated FRP plate subjected to the impact of foreign object and presented the stress and strain distribution through the thickness during impact. Choi and Chang [4] studied the impact damage on graphite/epoxy laminated composites caused by a low velocity impact in terms of /$  see front matter Ó 6 Elsevier Ltd. All rights reserved. doi:1.116/j.matdes
2 T. Roy, D. Chakraborty / Materials and Design 9 (8) matrix cracking and delamination resulting from a point node impact. Lam and Sathiyamoorthy [5] presented a theoretical method to analyze the impact dynamics of a system, which consists of laminated beam, subjected to the impact of multiple spherical masses. Duan and Ye [6] developed a 3D finite element model incorporating frictional contact for studying the delamination at the interfaces due to low velocity impact. Li et al. [7] investigated the effect of plate size, boundary condition, impactor mass and velocity on delamination size. Tay et al. [8] applied element failure concepts for dynamic fracture and delamination in the low velocity impact of composites. Alsan et al. [9] conducted experiments and performed 3D finite element analysis to evaluate the delamination damage of Eglass/epoxy laminated composites subjected to low velocity impact and evaluated the delamination at various interfaces. Shyr and Pan [1] investigated the damage characteristics and failure strengths of composite laminates at low velocity impact by performing experiments using a guided drop weight test rig and observed that the fiber breakage had occurred prior to the major damage. Moura and Goncalves [11] modelled the interaction between matrix cracking and delamination in carbon epoxy laminates under low velocity impact. They developed a numerical model based on an interface finite element compatible with 3D solid elements. Choi and Lim [1] suggested that linearized contact law could be well applied to low velocity impact analysis of composite laminates. Tay and Gosse [13] reported the use of element failure concepts with a recent failure criterion called the strain invariant failure theory (SIFT) in the direction of damage progression in a composite laminate subjected to threepoint bend. Zou et al. [14] proposed a method for modeling the damage of multiple delaminations and transverse matrix cracking in laminated composites due to low velocity lateral impact. Allix and Blanchard [15] analyzed the mesomodelling of delamination towards industrial applications and presented a structural failure criterion in order to predict which levels of damage and delamination are critical. Hosseizadeh et al. [16] analyzed the damage behavior of fiber reinforced composite plates subjected to drop weight impacts. In the direction of improving the impact response by hybridization, Adams and Zimerman [17] showed that the impact performance of graphite/epoxy laminate could be improved by hybridization with discrete plies of polyethylene/epoxy. Jang et al. [18] showed that addition of nylon/epoxy, polyester/epoxy and polyethylene/epoxy led to improvement of impact resistance of graphite/epoxy according to stacking sequence. Lee et al. [19] studied the effect of hybridizing graphite/epoxy with glass/epoxy and kevlar/epoxy on the impact resistance. Literature review reveals that many works have already been done in the area of impact response of laminated composite structures and it still remains an important area of research. Hybrid laminates have been studied by many researchers for improvement of impact resistance of laminated composite structures. Laminated plates containing holes or cutouts have been studied very extensively in the literature [3 5]. However, most of these studies concentrated on tensile and compressive loading. Relatively fewer studies have been conducted on the impact failure of composite plates containing holes or cutouts. Composite plates containing holes are more prone to delamination initiating at the interface near the edges of the holes. Therefore, the present paper aims at studying the response of the single and hybrid laminated composite plates with holes due to low velocity impact and also studying the chances of delamination at the interfaces of such laminates.. Finite element formulation Fig. 1 shows a laminated FRP composite plate of length L, width W and thickness h consisting of N laminae of different fiber orientation, clamped at its four edges and impacted by a spherical impactor of mass m and striking with an initial velocity of V Noded layered solid element Threedimensional 8noded isoparametric layered solid elements were used for modeling of the laminated plate (Fig. ). The shape functions defining the geometry and displacement are N i ¼ 1 8 ð1 þ rr iþð1 þ ss i Þð1 þ tt i Þ; i ¼ 1; ; 3;...; 8 ð1þ where r, s, t are natural coordinates and r i, s i, t i are the values of natural coordinates for the ith node. Extra shape functions are introduced to the general 8noded solid element in order to simulate the flexural response and they are P 1 ¼ð1 r Þ P ¼ð1 s Þ P 3 ¼ð1 t Þ ðþ The displacement variation within the element is thus Fig. 1. Impact on a laminated plate with holes by spherical impactor.
3 16 T. Roy, D. Chakraborty / Materials and Design 9 (8) Gauss quadrature scheme is applied to evaluate the above integration. The stiffness matrix of Eq. (8) is reduced to 4 4 using static condensation technique. Element mass matrix is evaluated as Z ½M e Š¼ ½NŠ T q½nšdv ð9þ V m.. Contact impact modeling 8 9 >< u >= fdg ¼ v >: >; ¼ X8 w i¼1 N i 8 >< u i v i >: w 9 >= þ½pšfwg ð3þ >; where 3 P 1 P P ½PŠ ¼4 P 1 P P 3 5 P 1 P P 3 and ½WŠ T ¼ ½W 1 W W 3 W 4 W 5 W 6 W 7 W 8 W 9 Š The stiffness matrix is calculated as ½KŠ ¼ Let Z 1 Z 1 Z 1 Gðr; s; tþ ¼½BŠ T ½CŠ½BŠjJj then ½KŠ ¼ Z 1 Z 1 Z 1 ½BŠ T ½CŠ½BŠjJjdr dsdt Gðr; s; tþdr dsdt For an element having N layers in the thickness direction (Fig. ), T ¼ XN k¼1 t k Fig.. 8noded layered element. where T is the total thickness of the element and t k is the thickness of the kth layer of the element. Taking a parameter te[,t] and changing the limits ½KŠ ¼ Z 1 Z 1 X N Z t k t 1 k Gðr; s; tþdr dsdt ð8þ T k¼1 where t is function of thickness over the layer. ð4þ ð5þ ð6þ ð7þ Dynamic equation governing the impact problem (neglecting damping) at time t + Dt is ½MŠf dg tþdt þ½kšfdg tþdt ¼fFg tþdt ð1þ where [M] and [K] are the mass and stiffness matrices and ff g; fdg; f dg; _ f dg are force, displacement, velocity and acceleration vectors for plate, respectively, at time t + Dt. Using Newmarkb method, Eq. (1) can be reduced to ½ bkšfdg tþdt ¼fbF g tþdt ð11þ where ½ bkš is the effective stiffness matrix and ½bF Š is the effective force vector and are defined as ½ bkš ¼ 1 UDt ½MŠþ½KŠ fbf g¼fhg t þffg tþdt fhg t 1 ¼½MŠ UDt fdgt þ 1 UDt f dgþ _ 1 U 1 f dg ð1þ ð13þ ð14þ where / and d are the Newmark constants. In Eq. (11), displacement, velocity and acceleration at time t are known at each point inside the plate and the unknown quantities in this equation are vector {d} t+dt and the force vector {F} t+dt. In the absence of preload, (11) becomes ½ bkšfdg tþdt ¼fHg t þfpg tþdt ð15þ where {P} is the contact force. The displacement vector {d} is expressed as the sum of the displacements due to the force {H} and the contact force {P} as fdg tþdt ¼fdg tþdt H þfdg tþdt P Eqs. (15) and (16) give ð16þ ½ bkšfdg tþdt H ¼fHg t ð17þ and ½ bkšfdg tþdt P ¼fPg tþdt ð18þ Writing {P} t+dt = f t+dt {U}, where f t+dt is the magnitude of contact force at time t + Dt, Eq. (18) yields ½ bkšfdg tþdt P ¼ f tþdt fug ð19þ and for a unit contact force (f t+dt =1)
4 T. Roy, D. Chakraborty / Materials and Design 9 (8) ½ bk Šfdg tþdt U ¼fUg ðþ where fdg tþdt U is the displacement caused by the unit contact force and d tþdt C ¼ d tþdt CH þ f tþdt d tþdt CU ð7þ Combining Eqs. () (7), the following expressions for the contact force are obtained: Z tþdt Z tþdt Z tþdt 1:5 f tþdt f ¼ j vdt þ dt dt dtþdt CH m f tþdt d tþdt CU during loading f tþdt ¼ f m R tþdt vdt þ R tþdt R tþdt f dt dt dtþdt m CH f tþdt d tþdt CU a a m a! :5 during unloading ð8þ fdg tþdt P ¼ f tþdt fdg tþdt U Eqs. (16) and (1) give fdg tþdt ¼fdg tþdt H þ f tþdt fdg tþdt U ð1þ ðþ Using Hertzian contact law, contact forces during loading and unloading are f tþdt ¼ jða tþdt Þ 1:5 during loading :5 during unloading f tþdt ¼ f m a tþdt a a m a ð3þ where j is the modified constant of the Hertz contact theory, a is the indentation depth, f m is the maximum force just before unloading, a m is the indentation depth corresponding to f m and a is the permanent indentation during loading and unloading process. Permanent indentation can be determined from the following expressions: a ¼ when a m < a cr " a ¼ a m 1 a # =5 cr ð4þ when a m > a cr a m Contact force at t + Dt, i.e. f t+dt, was calculated using Eq. (8) (during loading or during unloading) by Newton Raphson method. From the known value of contact force f t+dt, displacement vector {d} t+dt is calculated using Eq. (). Once the value of f t+dt is known, plate velocity, acceleration and then the stresses and strains at time t + Dt were calculated. This procedure has been repeated for each time step to get the displacement, stress and strain. The nodal stresses are obtained by using a leastsquare formulation proposed by Hinton and Campbell []. The extrapolated nodal stresses are obtained by ðr i Þ¼½ST Šðr J Þ ð9þ where r i and r j are nodal and Gauss point stresses, respectively, [ST] is the transformation matrix. For the present analysis, the transformation matrix from Gaussian stresses to extrapolated nodal stresses for threedimensional eight nodded layered brick element is obtained by ½ST Š¼ N 1 ðr j ; s j ; t j ÞN 1 ðr j ; s j ; t j Þ : : N 1 ðr j ; s j ; t j ÞN 8 ðr j ; s j ; t j Þ N ðr j ; s j ; t j ÞN 1 ðr j ; s j ; t j Þ : : N ðr j ; s j ; t j ÞN 8 ðr j ; s j ; t j Þ... : : N 8 ðr j ; s j ; t j ÞN 1 ðr j ; s j ; t j Þ : : N 8 ðr j ; s j ; t j ÞN 8 ðr j ; s j ; t j Þ 3 N 1 ðr I ; s I ; t I Þ : : N 1 ðr VIII ; s VIII ; t VIII Þ... : : : :... 5 N 8 ðr I ; s I ; t I Þ : : N 8 ðr VIII ; s VIII ; t VIII Þ where a cr is the critical indentation. a tþdt ¼ d tþdt S Here d tþdt S and d tþdt C d tþdt C ð5þ is the position of the center point of the impactor is the displacement of the center of the mid surface of the plate in the direction of impact. At time t + Dt, the magnitude of d tþdt S can be determined by Newton s second law as d tþdt S ¼ Z tþdt vdt þ Using Eq. (), we have Z tþdt Z tþdt f dt dt m ð6þ where VIII is the number of Gauss points..3. Delamination at the interface In order to assess delamination initiation at the interface, the criterion proposed by Choi et al. [1] for impact induced delamination has been used in the present work. The criterion is D a r n 4 yz þ rnþ1 S n i xz S nþ1 i! þ rnþ1 yy Y nþ1! 3 5 ¼ e D ð3þ
5 18 T. Roy, D. Chakraborty / Materials and Design 9 (8) if e D P 1 failure e D 6 1 no failure Y n ¼ Y n ten if r yy P Y n ¼ Y n c if r yy 6 where D a is an empirical constant which has to be determined from the experiment, which has been taken as 1.8 as suggested by Choi et al. [4]. r xz is averaged interlaminar stress within the nth interface, which can be expressed as r n xz ¼ 1 h n Z tn t n r xz dt where t n and t n are upper and lower interfaces of nth ply in the laminate and h n is the thickness of the ply. 3. Results and discussion 3.1. Validation Based on the contact impact finite element formulation above, a computer code has been developed in C language for the present study. In order to verify the FE code developed, the following parameters were used for a steel ball impacting at the center of an isotropic plate. Plate dimensions:...8 m 3 with the four edges clamped; Impactor (steel ball) diameter:. m; Velocity of the impactor: 1 m/s; Steel properties: E = 1 9 N/m, G = N/m, t =.5, a cr =.1 m, density = 784 Kg/m 3. It has been observed that for a mesh size of (8 elements), and a time step of Dt = 1ls, an excellent agreement has been achieved with the analytical solution of Karas []. This is shown in Fig. 3. The code has also been validated for the impact of aluminum sphere on a [/ 45/45/9] S graphite/epoxy laminate, and excellent agreement on contact force, displacements, velocities of plate and impactor has been obtained with already published results of Wu and Chang [3]. Fig. 4 only shows the contact force history of such a graphite/epoxy laminate. Fig. 4. Contact force using present code with mesh size for impact of aluminum sphere on [/ 45/+45/9] S. 3.. Transverse impact on a laminate with holes A square laminated composite plate of length and width equal to 8 mm and thickness of 3 mm has been considered in the present study. The plate contains two circular holes of 4 mm diameter and is symmetrically placed with respect to the center of the plate. The centertocenter distance of the holes is mm. Threedimensional 8noded layered elements have been used to model the plate with fine refinement near the holes. Fig. 5 shows the template of a typical 3D FE mesh of the above model. Total number of elements in the FE model were 18 and the number of nodes was 919. Three types of laminates have been analyzed to assess their comparative performance in terms of impact response as well as the impact induced delamination at the interface. In the present case, [/ 45/45/9] S laminate has been considered. The laminate actually consists of four sub laminates each having a stacking sequence of [/ 45/45/9]. Three different laminates viz. GGGG, KGGK1 and KGGK have been analyzed to study their impact responses and the effect of hybridization on the impact response. Here, GGGG stands for [ G /45 G /45 G /9 G ] S, KGGK1 stands for [ K / 45 G /45 G /9 G / G / 45 G /45 G /9 G ] S and KGGK indicates [ K / 45 K /45 K /9 K / G / 45 G /45 G /9 G ] S where K and Fig. 3. Contact force compared with Karas solution [] with mesh size. Fig. 5. Template of 3D FE mesh of the plate with holes.
6 T. Roy, D. Chakraborty / Materials and Design 9 (8) Table 1 Materials properties for graphite/epoxy and kevlar/epoxy Lamina material property Graphite/ epoxy (G) Aramid/ epoxy (K) Critical indentation, a cr 8.64e 5 m 1.16e 4 m Longitudinal Young s 181 GPa 76 GPa modulus, E xx Transverse Young s modulus, E yy 1.3 GPa 5.5 GPa Shear modulus in x y 7.17 GPa.3 GPa direction, G xy Poisson s ratio in x y direction,.8.34 t xy Poisson s ratio in y z direction, t yz.8.34 Density 16 kg/m kg/m 3 Allowable longitudinal tensile 15 MPa 14 MPa stress, X t Allowable longitudinal 15 MPa 35 MPa compressive stress, X c Allowable transverse tensile 4 MPa 1 MPa stress, Y t Allowable transverse compressive 46 MPa 53 MPa stress, Y c Allowable inplane shear stress, S i 68 MPa 34 MPa Contact coeficient, j e8 N m e8 N m.5 G stand for kevlar/epoxy and graphite/epoxy lamina, respectively. The laminate is assumed to be clamped along all the four edges and impacted at the center by a 1.7 mm diameter aluminum sphere at a velocity of 9 m/s. The material properties used for the above calculations are listed in Table 1. Fig. 6 shows the contact force history for different laminates when impacted by the spherical aluminum impactor at 9 m/s. It could be clearly observed from this figure that magnitude of contact force is maximum for GGGG laminate while it is minimum for KGGK laminate. Contact force magnitude for KGGK1 hybrid laminate lies in between. It could also be observed that even though reloading occurs for all the three types of laminates, contact duration is much less in the case of graphite/epoxy laminate (GGGG) compared to that in the case of other two laminates. So, introduction of kevlar/epoxy increases the flexibility of the laminate compared to graphite/epoxy Fig. 7. Comparison of plate displacement for different laminates at 9 m/s impact velocity. Fig. 8. Comparison of impactor displacement for different laminates at 9 m/s impact velocity. laminates. Fig. 7 shows the plate displacement and as expected plate displacement is minimum in the case of graphite/epoxy (GGGG) and increases with the inclusion of kevlar/epoxy plies in the laminates. Fig. 8 shows the impactor displacement history and in consistent with contact force, rebound is maximum in case of graphite/epoxy. Impactor velocity history is shown in Fig. 9. Fig. 6. Comparison of contact force for different laminates at 9 m/s impact velocity. Fig. 9. Comparison of impactor velocity for different laminates at 9 m/s impact velocity.
7 13 T. Roy, D. Chakraborty / Materials and Design 9 (8) Fig. 1. Delamination size in the interfaces of single laminated plate (GGGG). Fig. 11. Delamination size in the interfaces of hybrid laminated plate (KGGK1).
8 T. Roy, D. Chakraborty / Materials and Design 9 (8) Using the stress based delamination criterion, delaminations at the interfaces have been assessed for different laminates subjected to the impact of aluminum sphere at 9 m/s. Fig. 1 shows that after 6 ls, delaminations occur only at three interfaces in the case of GGGG laminate. Fig. 11 shows that after 6 ls, delaminations occur only at four Fig. 1. Delamination size in the interfaces of hybrid laminated plate (KGGK).
9 13 T. Roy, D. Chakraborty / Materials and Design 9 (8) interfaces in the case of KGGK1 laminate. Fig. 1 shows that delaminations occur at as many as seven interfaces in case of KGGK laminate. The extent of delamination at a particular interface is highest in the case of KGGK laminate and lowest in the case of GGGG laminate and in the case of KGGK1 the extent of delamination is in between. The reason for more delaminations in case of KGGK1 and KGGK laminates compared to GGGG laminate is that the interfacial shear and normal strengths of graphite/epoxy is higher compared to that of kevlar/epoxy. Thus even though providing a kevlar/epoxy at the outer layer prevents the laminate from failure at the contact point due to low magnitude of contact force and contact stress, chances of delamination at the interface increase. From Figs. 1 1 which show delaminations at the interface of the laminates, it is clear that due to the presence of holes in the laminate, delaminations initiate from the vicinity of holes at different interfaces. It could also be observed that delamination propagates from the inner edges of holes towards impact point and from outer edges towards the edges of the plate with some specific direction. The direction of delamination at interfaces 1 and follows the direction of fiber in the ply below the interface, which agrees with already published observations. It could be observed from the figures that in the case of GGGG and KGGK1, delaminations occur only at the tensile side of the plate but in the case of KGGK, delamaninations occur also at the interfaces located in the compression side of the plate showing that the interfaces in the KGGK are more susceptible to delamination under impact loading. 4. Conclusions Threedimensional transient dynamic finite element analysis has been done to analyze the response of single material (graphite/epoxy) and hybrid (graphite/epoxy kevlar/epoxy) laminates having holes in it. Stress based delamination criterion has been used to assess the chances of impact induced delamination from the vicinity of the holes. From the present study, it is quite clear that delaminations initiate at the interface from the inner free edges of the holes and with time, delaminations from two holes meet each other forming a big delamination area. It is evident from the present study that kevlar/epoxy graphite/epoxy hybrid laminate is more flexible compared to only graphite/epoxy laminates. Even though kevlar/epoxy hybridization on graphite/epoxy laminate leads to reduced contact force and hence more impact resistance in terms of failure due to contact stresses, but the chances of delamination at the interfaces increase. References [1] Sun CT, Chattopadhyay S. Dynamic response of anisotropic laminated plates under initial stress to impact of a mass. J Appl Mech 1975;4: [] Sun CT, Chen JK. On the impact of initially stressed composite laminates. J Compos Mater 1985;19: [3] Wu H, Yung T, Chang FK. Transient dynamic analysis of laminated composite plate subjected to transverse impact. Comput Struct 1989;31: [4] Choi HY, Chang FK. A model for predicting damage in graphite/ epoxy laminated composite resulting from lowvelocity impact. J Compos Mater 199;6(14): [5] Lam KY, Sathiyamoorthy TS. Response composite beams under low velocity impact of multiple masses. Compos Struct 1999;44:5. [6] Duan SH, Ye TQ. Three dimensional frictional dynamic contact analysis for predicting low velocity impact damage in composites. Adv Eng Software ;33:9 15. [7] Li CF, Hu N, Cheng JG, Fukunaga H, Sekine H. Lowvelocity impactinduced damage of continuous fiberreinforced composites laminates. Part II. Verification and numerical investigation. Compos Part A ;33: [8] Tay TE, Tan VBC, Deng M. Elementfailure concepts for dynamic fracture and delamination in lowvelocity impact of composites. Int J Solids Struct 3;4: [9] Alsan Z, Karakuzu R, Okutan B. Response of laminated composite plates under low velocity impact loading. Compos Struct 3;59: [1] Shyr TW, Pan YH. Impact resistance and damage characteristics of composite laminates. Compos Struct 3;6: [11] Moura MFSF, Goncalves JPM. Modelling the interaction between matrix cracking and delamination in carbon epoxy laminates under low velocity impact. Compos Sci Technol 4;64:11 7. [1] Choi IH, Lim CH. Low velocity impact analysis of composite laminates using linearized contact law. Compos Struct 4;66: [13] Tay TE, Tan SHN, Tan VBC, Gosse JH. Damage progression by the elementfailure method (EFM) and strain invariant failure theory (SIFT). Compos Sci Technol 5;65: [14] Li S, Reid SR, Zou Z. Modelling damage of multiple delaminations and transverse matrix cracking in laminated composites due to low velocity lateral impact. Compos Sci Technol 6;66: [15] Allix O, Blanchard L. Mesomodelling of delamination: towards industrial applications. Compos Sci Technol 6;66: [16] Hosseinzdeh R, Shokrieh MM, Lessard L. Damage behavior of reinforced composite plates subjected to drop weight impacts. Compos Sci Technol 6;66:61 8. [17] Adams DF, Zimmerman RS. Static and impact performance of polyethylene fiber/graphite hybrid composites. SAMPE J. 1986;:1 6. [18] Jang BZ, Chen LC, Wang CZ, Lin HT, Zee RH. Impact resistance and energy absorption mechanism in hybrid composites. Compos Sci Technol 1989;34: [19] Lee YShin, Kang KHee, Park O. Response of hybrid laminated composite plates under lowvelocity impact. Compos Struct 1997;65: [] Hinton E, Champbell JS. Local and global smoothing of discontinuous finite element functions using a least squares method. Int J Numer Meth Eng 1974;8: [1] Choi HY, HisYoung TW, Chang FK. A new approach towards understanding damage mechanism and mechanics of laminated composites due to low velocity impact: Part II analysis. J Compos Mater 1991;5: [] Karas K. Platten Unter Seitchem stoss. Ing Arch 1939;1:37 5. [3] Awerbuch JA, Madhukar MS. Notched strength of composite laminate: prediction and experiments a review. J Reinf Plast Comp 1985;4: [4] Chang FK, Chang KY. Post failure analysis of Bolted Composite joints in tension or shearout mode failure. J Compos Mater 1987;1: [5] Chang FK, Lessard LB. Damage tolerance of laminated composites containing an open hole and subjected to compressive loadings: Part I analysis. J Compos Mater 1991;5:3 43.
ISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationFLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationSIMULATION OF BOND FAILURE IN RC BEAMS STRENGTHENED WITH FRP SHEETS SUBJECTED TO DYNAMIC/IMPACT LOADINGS
Proceedings of International Symposium on Bond Behaviour of FRP in Structures (BBFS 005) Chen and Teng (eds) 005 International Institute for FRP in Construction SIMULATION OF BOND FAILURE IN RC BEAMS STRENGTHENED
More informationDynamic mixedmode I/II delamination fracture and energy release rate of unidirectional graphite/epoxy composites
Engineering Fracture Mechanics 7 (5) 53 558 www.elsevier.com/locate/engfracmech Dynamic mixedmode I/II delamination fracture and energy release rate of unidirectional graphite/epoxy composites Sylvanus
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationA FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
TRENDS IN COMPUTATIONAL STRUCTURAL MECHANICS W.A. Wall, K.U. Bletzinger and K. Schweizerhof (Eds.) c CIMNE, Barcelona, Spain 2001 A FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationOPTIMAL DESIGN OF COMPOSITE INSERTS FOR A HYBRID ULTRACENTRIFUGE ROTOR
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS OPTIMAL DESIGN OF COMPOSITE INSERTS Hak Gu Lee 1*, Jisang Park 1, Ji Hoon Kim 1 1 Composite Materials Group, KIMS, Changwon, Korea * Corresponding
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationDetermination of the Shear Buckling Load of a Large Polymer Composite ISection Using Strain and Displacement Sensors
Sensors 2012, 12, 1602416036; doi:10.3390/s121216024 Article OPEN ACCESS sensors ISSN 14248220 www.mdpi.com/journal/sensors Determination of the Shear Buckling Load of a Large Polymer Composite ISection
More informationTransactions on Engineering Sciences vol 6, 1994 WIT Press, ISSN
Strain energy release rate calculation from 3D singularity finite elements M.M. Abdel Wahab, G. de Roeck Department of Civil Engineering, Katholieke Universiteit, Leuven, B3001 Heverlee, Belgium ABSTRACT
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationEFFECT OF SHEAR REINFORCEMENT ON FAILURE MODE OF RC BRIDGE PIERS SUBJECTED TO STRONG EARTHQUAKE MOTIONS
EFFECT OF SHEAR REINFORCEMENT ON FAILURE MODE OF RC BRIDGE PIERS SUBJECTED TO STRONG EARTHQUAKE MOTIONS Atsuhiko MACHIDA And Khairy H ABDELKAREEM SUMMARY Nonlinear D FEM was utilized to carry out inelastic
More informationBALLISTIC IMPACT MODELING OF COMPOSITE MATERIALS
7 th International LSDYNA Users Conference Penetration/Explosive BALLISTIC IMPACT MODELING OF COMPOSITE MATERIALS ChianFong Yen Materials Sciences Corporation 5 Office Center Drive Fort Washington, PA
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationEXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES
EXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES D. Kakogiannis 1, D. Van Hemelrijck 1, J. Wastiels 1, S. Palanivelu 2, W. Van Paepegem 2, K. De Wolf 3, J.
More informationNumerical modelling of induced tensile stresses in rock in response to impact loading
Numerical modelling of induced tensile stresses in rock in response to impact loading M.T. Mnisi, D.P. Roberts and J.S. Kuijpers Council for Scientific and Industrial Research (CSIR): Natural Resources
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationStresses and Displacements in Functionally Graded Materials of SemiInfinite Extent Induced by Rectangular Loadings
Materials 2012, 5, 210226; doi:10.3390/ma5020210 Article OPEN ACCESS materials ISSN 19961944 www.mdpi.com/journal/materials Stresses and Displacements in Functionally Graded Materials of SemiInfinite
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationThis is a publisherdeposited version published in: Eprints ID: 4094
This is a publisherdeposited version published in: http://oatao.univtoulouse.fr/ Eprints ID: 4094 To cite this document: WEISS Ambrosius, TRABELSI Walid, MICHEL Laurent, BARRAU JeanJacques, MAHDI Stéphane.
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationDamage in wovenfabric composites subjected to lowvelocity impact
Damage in wovenfabric composites subjected to lowvelocity impact N.K. Naik*, Y. Chandra Sekher, Sailendra Meduri Aerospace Engineering Department, Indian Institute of Technology, Powai, Mumbai400 076,
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationEffect of Strain Hardening on Unloading of a Deformable Sphere Loaded against a Rigid Flat A Finite Element Study
Effect of Strain Hardening on Unloading of a Deformable Sphere Loaded against a Rigid Flat A Finite Element Study Biplab Chatterjee, Prasanta Sahoo 1 Department of Mechanical Engineering, Jadavpur University
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationGeometrydependent MITC method for a 2node isobeam element
Structural Engineering and Mechanics, Vol. 9, No. (8) 33 Geometrydependent MITC method for a node isobeam element PhillSeung Lee Samsung Heavy Industries, Seocho, Seoul 37857, Korea HyuChun Noh
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More information1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor.
Elasticity Homework Problems 2014 Section 1. The Strain Tensor. 1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor. 2. Given a steel bar compressed with a deformation
More information2D damping predictions of fiber composite plates: Layup effects
Available online at www.sciencedirect.com Composites Science and Technology 68 (2008) 727 733 COMPOSITES SCIENCE AND TECHNOLOGY www.elsevier.com/locate/compscitech 2D damping predictions of fiber composite
More informationSoil Dynamics and Earthquake Engineering
Soil Dynamics and Earthquake Engineering 30 (2010) 1361 1376 Contents lists available at ScienceDirect Soil Dynamics and Earthquake Engineering journal homepage: www.elsevier.com/locate/soildyn Finite
More informationVORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS
The 4 th World Conference on Earthquake Engineering October 7, 008, Beijing, China VORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS K.
More informationA Piezoelectric Screw Dislocation Interacting with an Elliptical Piezoelectric Inhomogeneity Containing a Confocal Elliptical Rigid Core
Commun. Theor. Phys. 56 774 778 Vol. 56, No. 4, October 5, A Piezoelectric Screw Dislocation Interacting with an Elliptical Piezoelectric Inhomogeneity Containing a Confocal Elliptical Rigid Core JIANG
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationTensile Stress Acoustic Constants of Unidirectional Graphite/Epoxy Composites
Tensile Stress Acoustic Constants of Unidirectional Graphite/Epoxy Composites Journal of Reinforced Plastics and Composites, Vol. 9 (March, 1990) pp. 127133 W. H. PROSSER NASA Langley Research Center
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationModeling and analysis of the electromechanical behavior of surfacebonded piezoelectric actuators using finite element method
Modeling and analysis of the electromechanical behavior of surfacebonded piezoelectric actuators using finite element method Huangchao Yu and Xiaodong Wang Abstract Piezoelectric actuators have been widely
More informationThe Local Web Buckling Strength of Coped Steel IBeam. ABSTRACT : When a beam flange is coped to allow clearance at the
The Local Web Buckling Strength of Coped Steel IBeam Michael C. H. Yam 1 Member, ASCE Angus C. C. Lam Associate Member, ASCE, V. P. IU and J. J. R. Cheng 3 Members, ASCE ABSTRACT : When a beam flange
More informationModeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress
Modeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress Authors Marco ANGHILERI * LuigiM L CASTELLETTI * Andrea MILANESE * and Andrea SEMBOLONI * Affiliation * Politecnico
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationHEALTH MONITORING OF PLATE STRUCTURE USING PIEZO ELECTRIC PATCHES AND CURVATURE MODE SHAPE
ISSN (Online) : 23198753 ISSN (Print) : 23476710 International Journal of Innovative Research in Science, Engineering and Technology An ISO 3297: 2007 Certified Organization, Volume 2, Special Issue
More informationU.S. South America Workshop. Mechanics and Advanced Materials Research and Education. Rio de Janeiro, Brazil. August 2 6, Steven L.
Computational Modeling of Composite and Functionally Graded Materials U.S. South America Workshop Mechanics and Advanced Materials Research and Education Rio de Janeiro, Brazil August 2 6, 2002 Steven
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationFinite ElementBased Failure Models for Carbon/Epoxy Tape Composites
Finite ElementBased Failure Models for Carbon/Epoxy Tape Composites A Master Thesis Presented to The Academic Faculty by Guillaume Seon In Partial Fulfillment of the Requirements for the Degree Master
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationFrequency Response of Composite Laminates at Various Boundary Conditions
International Journal of Engineering Science Invention (IJESI) ISSN (Online): 2319 6734, ISSN (Print): 2319 6726 www.ijesi.org ǁ PP.1115 Frequency Response of Composite Laminates at Various Boundary Conditions
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationStatic & Dynamic. Analysis of Structures. Edward L.Wilson. University of California, Berkeley. Fourth Edition. Professor Emeritus of Civil Engineering
Static & Dynamic Analysis of Structures A Physical Approach With Emphasis on Earthquake Engineering Edward LWilson Professor Emeritus of Civil Engineering University of California, Berkeley Fourth Edition
More informationNonlinear Analysis of Reinforced Concrete Shells Subjected to Impact Loads
Transactions of the 7 th International Conference on Structural Mechanics in Reactor Technology (SMiRT 7) Prague, Czech Republic, August 7, 00 Paper # J0 Nonlinear Analysis of Reinforced Concrete Shells
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationShear Strength of Slender Reinforced Concrete Beams without Web Reinforcement
RESEARCH ARTICLE OPEN ACCESS Shear Strength of Slender Reinforced Concrete Beams without Web Reinforcement Prof. R.S. Chavan*, Dr. P.M. Pawar ** (Department of Civil Engineering, Solapur University, Solapur)
More informationDYNAMIC ANALYSIS OF PILES IN SAND BASED ON SOILPILE INTERACTION
October 117,, Beijing, China DYNAMIC ANALYSIS OF PILES IN SAND BASED ON SOILPILE INTERACTION Mohammad M. Ahmadi 1 and Mahdi Ehsani 1 Assistant Professor, Dept. of Civil Engineering, Geotechnical Group,
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationInternational Conference on Mechanics and Civil Engineering (ICMCE 2014)
International Conference on Mechanics and Civil Engineering (ICMCE 2014) Parametric Design and Experimental Study for Weak Area Structure of Circle Composite Fragile Cover Ran CAO 1,a, GuangMing ZHOU
More informationFinite element simulation of residual stresses in laser heating
IAS200866546ST Finite element simulation of residual stresses in laser heating G. H. Farrahi 1, M. Sistaninia 2, H. Moeinoddini 3 1,2School of Mechanical Engineering, Sharif University of Technology,
More informationTHE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE
Journal of Applied Mathematics and Computational Mechanics 013, 1(4), 131 THE INFLUENCE OF THERMAL ACTIONS AND COMPLEX SUPPORT CONDITIONS ON THE MECHANICAL STATE OF SANDWICH STRUCTURE Jolanta Błaszczuk
More informationComputers and Structures
Computers and Structures 87 (2009) 1451 1460 Contents lists available at ScienceDirect Computers and Structures journal homepage: www.elsevier.com/locate/compstruc A triangular sixnode shell element DoNyun
More informationIntensity (a.u.) Intensity (a.u.) Raman Shift (cm 1 ) Oxygen plasma. 6 cm. 9 cm. 1mm. Singlelayer graphene sheet. 10mm. 14 cm
Intensity (a.u.) Intensity (a.u.) a Oxygen plasma b 6 cm 1mm 10mm Singlelayer graphene sheet 14 cm 9 cm Flipped Si/SiO 2 Patterned chip Plasmacleaned glass slides c d After 1 sec normal Oxygen plasma
More information